This is the 11th lecture of this course and the last lecture on the topic of Equilibrium Carrier Concentration.


 Egbert Lambert
 2 years ago
 Views:
Transcription
1 Solid State Devices Dr. S. Karmalkar Department of Electronics and Communication Engineering Indian Institute of Technology, Madras Lecture  11 Equilibrium Carrier Concentration (Contd.) This is the 11th lecture of this course and the last lecture on the topic of Equilibrium Carrier Concentration. (Refer Slide Time: 01:09) In yesterday s class, I explained the behavior of concentration in an extrinsic semiconductor as a function of reciprocal of temperature that is the majority carrier concentration.
2 (Refer Slide Time: 01:30) So we have explained this particular slide. More specifically we have explained how in the different regions here for example, this is extrinsic range, this is the partial ionization range and this is the intrinsic range. How in these three ranges the concentration behaves? We have shown, for example, in the intrinsic range, this range here, your concentration is the same as intrinsic concentration given as square root of N c N v e power x minus (Eg by 2KT). (Refer Slide Time: 02:03) Please note that this formula will hold good in the range where the concentration is exactly equal to the intrinsic concentration. Somewhere near the border obviously this
3 formula will not be valid, we will have to make a more accurate estimation. Similarly, analogous to this range in the partial ionization range which is this particular range the formula is 1 square root of N c N d (e power x) minus (Eion by 2KT) where Eion is ionization energy. We have shown this result by considering the band diagram and the analogy between the situation here and the situation in the intrinsic range. Then in the extrinsic range which is a range of interest to us from the point of view of device operation the concentration is equal to the doping level. This is when considering an n type semiconductor. Now note that the concentration here is on a log scale and this is on a reciprocal of temperature scale. Today we will see how to calculate the intrinsic temperature and how to calculate the Fermilevel and then we will have a solved example to illustrate how Fermilevel and concentrations can be calculated for specific situations. Let us look at the intrinsic temperature T i. This particular temperature depends on the border between extrinsic range and the intrinsic range. So how do you define the intrinsic temperature? We can define the intrinsic range temperature using the linear plot of concentration versus temperature. (Refer Slide Time: 03:52) On the linear plot the definition of the intrinsic concentration will be seen much more easily, so this plot is something like this where this is the intrinsic concentration n i and this is the total contribution because of the thermal generation as well as impurity ionization. I will remove this portion and show only the contribution because of impurity ionization N d. This is the curve representing contribution of the impurity and this is the term representing the effect of thermal generation and more specifically this is intrinsic concentration. Now this is the point where the intrinsic concentration becomes equal to the doping T i, this point is defined as the intrinsic point.
4 So you define intrinsic point in terms of the doping level and intrinsic concentration where N d is equal to n i.. The formula therefore would be N d is equal to n i at T i is equal to square root of N c N v e to the power x(minus Eg by 2KT i ) and when you transform you get T i is equal to Eg by 2K into ln square root of N c N v by N d. This is obtained from this equation by transformation. Whenever we derive a formula of this type we must check qualitatively whether the formula is correct and whether all these terms are in the correct position. Two important physical parameters on which T i the intrinsic temperature depends is the energy gap Eg and doping level N d. According to this formula T i should increase with energy gap. This is physically correct because if your energy gap is large you must go to higher temperatures to generate the n i corresponding to the doping level. Similarly, according to this formula again if your N d is large the denominator is small and therefore this is large which means that T i is large. This is also correct because if N d is large you have to go to higher temperatures to generate n i. So qualitatively it appears that the formula is correct. In terms of this formula one can calculate the intrinsic temperatures. Let us see what kind of values result. (Refer Slide Time: 07:31) Here the intrinsic temperature has been shown for gallium arsenide and silicon. It is because gallium arsenide has higher energy gap of 1.4 electron volts it has higher intrinsic temperature as compared to silicon whose energy gap is 1.1 electron volts. Let us look at some values at 10 power 13 by cm cube doping level where the intrinsic temperature for silicon is around 450K roughly whereas that of gallium arsenide is about 650K. The gallium arsenide intrinsic temperature is higher by about 200K. You come to about 2(10 power 15) by cm cube doping level, the gallium arsenide intrinsic temperature is 1200K whereas that of silicon is about 700K. That is how the intrinsic temperature depends on the energy gap of the semiconductor and doping level. The intrinsic temperature is important in deciding the extrinsic range. So, if you want to use a device at
5 higher temperatures or for some reason if the device is going to dissipate large amount of power like a power device and therefore its temperature is likely to rise then it is clear that semiconductors with higher energy gap are more suitable for such applications than semiconductors with lower energy gap. This is the importance of intrinsic temperature. (Refer Slide Time: 09:39) Now let us consider how to estimate the Fermilevel? We know that n 0, the equilibrium concentration on electrons is given by N c exp(minus E c minus E f minus by KT). So from here I can get the relation E f given by E c minus KT ln N c by n 0. Here n 0 is equal to N d if there is complete ionization. We are talking of the extrinsic range but more generally this is the relation. So this is how the Fermilevel can be located in terms of the electron concentration. You could locate the Fermilevel in terms of the whole concentration. For that instead of n 0 you will use the formula for p 0 where p 0 is equal to N v exponential of minus E f minus E v by KT which results in E f is equal to E v plus KT ln N v by P 0. So the Fermilevel is located above E v by this much value in terms of the whole concentration. Here this formula looks at the Fermilevel with respect to the band edges E c and E v. One can also locate the Fermilevel with respect to the intrinsic level of the Fermilevel in a pure or intrinsic semiconductor. This is important because you know that intrinsic semiconductor wwhole concentration is equal to electron concentration and Fermilevel is at the middle of the energy gap. In a doped semiconductor the concentration will deviate from the concentration in an intrinsic semiconductor depending on the doping and therefore the Fermilevel is deviating. So how much does a Fermilevel deviate from the position in the intrinsic semiconductor because of doping? We can relate E f to E i, how we do that? Look at this relation n 0 is equal to N c exponential minus E c minus E f by KT. In addition, we can write the relation n i is equal to N c exp of E c minus E i by KT it is a negative sign and now we can take the ratio of n 0 and n i.
6 (Refer Slide Time: 12:37) If you take the ratio of n 0 and n i then you will find that your relationship will be E f is equal to E i plus KT ln n 0 by n i. So if it is an ntype semiconductor then n 0 greater than n i. The Fermilevel is above E i ; One can similarly do the exercise in terms of whole concentration and you will get E f is equal to E i minus KT ln p 0 by p i. So the Fermilevel in a ptype semiconductor when p 0 greater than p i is below E i. This is how we can locate the Fermilevel in terms of the electron whole concentrations. Let us show this on an energy band diagram. (Refer Slide Time: 14:06)
7 This is E c, this is E v and this is E i suppose it is ntype semiconductor then this will be E f and it is above E i. So this difference E f minus E i is given by KT ln(n 0 by n i ) is this formula, so E f minus E i is equal to KT ln (n 0 by n i ). So alternately you can locate E f from the conduction band edge and this is given by KT ln(n c by n 0 ) which is this particular formula. So E c minus Ef you shift Ef this side it is KT ln(n c by n 0 ), this is ntype. Now you can similarly write relations for Fermilevel in a ptype semiconductor. This is n type. Now, using this formula if you estimate the Fermilevels in silicon for various boron doped and phosphorus doped crystals in the extrinsic range what kind of crystals you will have? So in the extrinsic level you can replace Nn 0 by N d for phosphorous doped silicon which is the doping level. So this is under the assumption of complete ionization of the impurity and neglect of the thermal generation. Here n 0 is approximately equal to N d in an ntype semi conductor in the extrinsic range. So we are interested in estimating Fermilevel in the extrinsic range because that is the range in which the devices operate. Therefore our relations would be E f is equal to E c minus kt ln N c by N d or alternately E f is equal to E v plus KT ln N v by N a and this will be in a ptype semiconductor, so this is the ntype, the Fermilevel in extrinsic range and this is for ptype. (Refer Slide Time: 16:57) Now you could also use the formula E f is equal to E i plus KT ln n 0 by n i so here n 0 will be replaced by N d for ntype and here p 0 will be replaced by N a and p i is nothing but n i so we could write p i or n i it does not make a difference. This is again ntype and this is ptype so you could use any of this formulae for ntype. When you make an estimation using this at room temperature the calculation looks something like this as shown in the slide here.
8 (Refer Slide Time: 18:03) So this is the Fermilevel plotted within the extrinsic range. So you find at higher temperatures this is Fermilevel plotted with respect to E i so E f minus E i this is for ntype silicon and this is for ptype silicon and the xaxis is temperature. So you have a behavior both as a function of temperature and doping. You find that in high temperatures the Fermilevel tends to the intrinsic level both for ntype as well as for ptype. The intrinsic temperature is higher for higher doping and that is why this particular Fermilevel here for 10 to the power 17 per cm cube doping has not yet reached the intrinsic level because the doping is higher. At the other end the Fermilevel for all doping levels tends to be at the middle of the region between the conduction band edge E c and the donor level for the ntype semi conductor. Let us understand this in terms of the diagram below.
9 (Refer Slide Time: 19:17) Qualitatively we located the Fermilevel in an ntype semiconductor as per this diagram. So, for T is equal to 0 the Fermilevel is at middle of E c and E d, it is at the midpoint of this difference here irrespective of the doping level. Now we did not derive this relation exactly but we showed that the Fermilevel in a ntype semi conductor at T is equal to 0 has to be above E d but below E c. Now if you make exact calculations using formulae and so on you will get it at the mid point here. So that is what is being shown here in the slide. Here these lines are tending towards that point. Now, similarly for ptype silicon they will tend towards these lines, these Fermilevels will tend towards the middle of the accepted level and the valence band edge. Now, to complete the understanding of this diagram, note that the E c and E v have also been shown to vary with temperature. So E c minus E v is the difference between E c and E v that is the energy gap seems to reduce with temperature. This is true for many semiconductors that the energy gap reduces with temperature. So what is shown in this slide is the variation for silicon because of the reduction in energy gap the intrinsic concentration that you calculate from the formula square root of N c N v e power x (minus Eg by 2KT) will be slightly higher than that you estimate assuming a constant energy gap of 1.12v. Hence that energy gap 1.1v is at 300k and for any other temperature if you want the energy gap you have to use this behavior which is there in some sort of a formula which you are not going to do derive in this course. After considering the Fermilevel now let us look at the topic of compensated semiconductors.
10 (Refer Slide Time: 21:40) Compensated semiconductors: In one of the previous classes in response to a question I had explained how we can predict the behavior of semiconductors in which you have both ptype and ntype impurities using the bond model. That is both phosphorous and boron doping. Now we want to look at the behavior from the energy band point of view. So specifically we had mentioned in that context that for compensated semiconductors your charge balance equation can be written as n o plus N a to the power minus is equal to p o plus N d power plus, here n 0 is electron concentration, p 0 is whole concentration, N a power minus is the ionized acceptor concentration, N d plus is the ionized donor concentration. So, according to this formula supposing you start with ntype semi conductor and you introduce acceptor impurities, so you start with a phosphorous doped semiconductor and you increase the concentration of boron impurity from 0 onwards, now what the behavior is like? You can predict that behavior using this formula n o is equal to p o plus N d to the power plus N a power minus. I am rewriting this balance equation like this which we have done in the context of the discussion on compensate semiconductors earlier. This clearly shows that your electron concentration starts reducing as you start raising N a to the power minus from 0 onwards. Let us understand this particular behavior from the energy band point of view. So what is happening? You have this E c E v and these are the donors in an ntype semi conductor.
11 (Refer Slide Time: 23:41) Let us say we are talking of the extrinsic range or we are working around room temperature and these donors are phosphorous so all of them are ionized. So N d power plus is actually N d this is shown here by these arrows here. Therefore each of these donors have given away an electron which has gone to the conduction band. Now there is another process that is the process of thermal generation which will be shown as an arrow going from valence band to conduction band and this is thermal generation and this is also present but we know that the contribution of this to the concentration around room temperature is very small so we will not bother about this but concentrate only on the impurity ionization. Supposing you add acceptor impurities what is going to happen? Here the number of positive signs in some way indicates the concentration of donor impurities. Thus smaller number of negative signs shows that N a less than N d. Now let us say that we have added these acceptor atoms and what is going to happen? Now, while discussing the energy band model we said that one of the postulates is that electrons occupy the lowest energy states available to them. The moment you have introduced the acceptor impurities you have introduced allowed states for the electrons here below this donor level. What is going to happen is the electrons from these donor levels instead of jumping up to conduction band they would find it more convenient to jump down on to this acceptor level. So each acceptor level is going to accept an electron from the donor impurity and so these electrons from donor impurity instead of becoming free will get trapped at the acceptors side. This is how the acceptor atoms are reducing the concentration of electrons in the ntype semiconductor. Now one can extend this logic and show that if N a becomes more than N d which means this will correspond to the picture like this. I will explain this line here to show that N a has become more than N d. So this is E c, E v, E d and this is E a the acceptor level. Now what
12 is going to happen is all these arrows will go away so electrons will jump down on to the acceptor side instead of jumping up from the impurity the donor level. So all these impurities have been totally compensated by the acceptor atoms and now these acceptor atoms are there which will accept an electron from the valence band edge and as a result will give raise to holes. Now the semiconductor has changed polarity and it has become ptype rather than ntype because it has now got holes. This is how one can look at the behavior of compensated semiconductors from the energy band point of view and understand the particular phenomenon of compensation. If your ntype doping is more than ptype doping you get an ntype semiconductor if your ptype doping is more than ntype doping you get a ptype semiconductor. After this we will solve a problem, a numerical example which will show us how carrier concentration is estimated and how the Fermilevel is located. (Refer Slide Time: 27:49) Now we shall illustrate some of the ideas related to Fermilevel and carrier concentration with the help of a numerical example. The example is the following: What are the majority and minority carrier concentrations in silicon doped with 10 to the power 16 cm cube atoms of boron and 5 into 10 to the power 15 cm cube atoms of phosphorous, at 300K and 600K? Check the assumptions made in the calculation. So basically we want to estimate carrier concentration in a compensated semiconductor at two different temperatures by checking the assumptions which have been made. Let us see the assumptions which we make.
13 (Refer Slide Time: 28:38) The assumptions that we make normally while estimating carrier concentration are: complete impurity ionization, negligible thermal generation and Boltzmann approximation. Let us see where these approximations or assumptions are made for simplifying the calculation. Let us start with the carrier concentration at 300K. (Refer Slide Time: 29:05) First we need to estimate the majority carrier concentration and for this we use the charge balance equation. We note that since the boron concentration of 10 to the power 16 cm cube is more than the phosphorous concentration of 5 into 10 to the power 15 it is a p type semiconductor. We write the charge balance equation as p p0 which is the hole
14 concentration in the ptype semiconductor which is equal to N a minus the ionized acceptor concentration minus the ionized donor concentration plus the concentration of thermally generated carriers which is also the minority carrier concentration (p p0 is equal to (N a minus N d to the power plus)plus n p0. When you make the assumption of complete impurity ionization this minus and plus signs drop out so that is a simplification. Further when you make the assumption of neglecting the thermal generation that is this particular term n p0 is much less than this term N a minus N d that is the meaning of neglecting thermal generation so we remove this term also. This is how your equation gets simplified for the majority carrier concentration and so the result is equal to 10 to the power 16 minus 5 into 10 to the power 15 which is equal to 5 minus 10 to the power 15 cm cube so that is the hole concentration. Now the electron concentration n p0 is equal to n i square by p p0. Now n i at 300K is 1.5 into 10 to the power 10 cm cube so (1.5 into 10 to the power 10) whole square by 5 into 10 to the power 15 and the result is 4.5 into 10 to the power 4 by cm cube which is the minority carrier concentration. Having obtained these concentrations now we must check the assumptions. For example, supposing we want to check the assumption of negligible thermal generation what does it mean? We need to check whether n p0 as obtained here is much less than N a minus N d which is obtained here so this is indeed the case. So since n p0 is equal to 44.5 into 10 to the power 4 less than N a minus N d is equal to 5 into 10 to the power 15 cm cube. Here also the unit is per cm cube hence thermal generation is negligible. We have to check the assumption of negligible thermal generation at 300K. Now how will you check the assumption of impurity ionization? Is N a to the power minus is equal to N a? Is N d to the power plus is equal to N d? To check that we will have to locate the Fermilevel because we know the fraction N a to the power minus by N a is the number of occupied states at the energy level E a. (Refer Slide Time: 33:05)
15 So this fraction is given by 1 by 1 plus exp (E a minus E f by KT). Similarly N d to the power plus by N d is the number of unoccupied states at the energy level E d. This is 1 minus 1 by 1 plus exp (E d minus E f by KT). E d is the donor level corresponding to N d, E a is an acceptor level corresponding to N a. If you know the location of Fermilevel then we can find out these fractions and check whether N a to the power minus by N a is equal to 1 and whether N d to the power plus by N d is either equal to or close to 1. Let us look at the energy band diagram. (Refer Slide Time: 34:27) That is something like this, this is E c and this is E v and this is E d donor level, this is acceptor level corresponding to boron so this is E a. Since it is a ptype semiconductor Fermilevel E f will be close to the valence band edge than conduction band edge that is away from the intrinsic level and this is E i. So let us say the Fermilevel is somewhere here, we do not know exactly where it is but we will now locate it shortly, it will be below E i. Since this is a ptype semiconductor it will be useful to locate the Fermilevel either with respect to the valence band edge or with respect to E i but not with respect to conduction band edge. So let us locate with respect to valence band edge that is we want to know what is this difference? From the formula we know that this difference is KT ln N v by p p0. This is where we are using the Boltzmann approximation now to estimate the location of the Fermilevel. Incidentally the Boltzmann approximation was also used when we estimated the minority carrier concentration from n i square by majority carrier concentration formula and this is because minority carrier concentration into majority carrier concentration is equal to N a square or p to the power n is equal to N a square where this particular relation comes only after we make a Boltzmann approximation. Coming back here the location of the Fermilevel with respect to E v can be obtained by using this formula KT ln N v by p p0. Once we know that we can make the calculation of
16 the ionized impurities because we know these distances E a minus E v is equal to volt. Similarly this difference is also volts. So if you want E d minus E f then it will be this difference and if you want E a minus E f it will correspond to this difference. These are the two differences we want. Once we know this difference we can estimate the other two. Now what is the value of this KT ln N v by p p0? p p0 we have estimated to be 5 into 10 to the power 15 by cm cube under our assumptions and N v is 10 to the power 19 divided by cm cube and this KT is equal to volts. So if you substitute all these values and then estimate this particular difference it will turn out to be equal to electron volts which is the difference. So as a result this difference is electron volts. Now we can try to estimate this relation N a to the power minus by N a which will be is equal to 1 by 1 plus exp (E a minus E f by KT). This will be 1 by 1 plus exponential minus by and this works out to 1 minus 2.78 into 10 to the power minus 3. So this 2.78 into 10 to the power minus 3 is very small compared to 1 so N a to the power minus by N a is approximately equal to 1 and complete ionization of acceptor impurities is justified. Now one can similarly do an estimation of N d to the power plus by N d. However we need not do a calculation again to check whether this is indeed close to 1 because you see E d minus E f by KT where E d minus E f is this difference which is definitely much larger than E f minus E a which means that this term here E d minus E f would be much greater than and therefore this term again would be much less than 2.78 into 10 to the power minus 3. So as a result we can definitely say if the acceptor impurities in a ptype semiconductor like boron doped semiconductor are ionized then definitely the donor impurities present in the ptype semiconductor will also be completely ionized. So we need not do a calculation again for the phosphorus atoms or donor impurities. With that we have checked and justified the assumption of complete ionization. Now is Boltzmann approximation justified because that is a third assumption we have made so that can also be seen very easily as E f minus E v is electron volts should be three times greater than KT. Now 3KT in this case at room temperature is electron volts. Since electron volts is greater than electron volts the Boltzmann approximation is justified and is valid. If the boron doping was higher slowly you can see from here that this E f will start moving close to E v and then there is a likelihood of the Boltzmann approximation getting violated. But as it is you see that Boltzmann approximation is justified. Now even before actually making accurate calculation of this particular fraction N a to the power minus by N a once we have located the Fermilevel here we can get a feel for the fact that the acceptor impurities and the donor impurities are fully ionized because E f is above E a, and using the FermiDirac fraction we know that most of the levels below E f will be occupied and most of the levels which are far away from E f on the top will be unoccupied. That is how donor impurities are fully ionized and acceptor impurities also are fully ionized once we locate the Fermilevel and even without making a numerical estimation.
17 Now one can repeat the same procedure for 600 Kelvin. However one thing you must note that we need not check again whether complete ionization will be justified at 600K by calculation because we know that at 300K if the impurities are ionized at 600K they will definitely be ionized. Similarly, even for the Boltzmann approximation one need not check again because you know that as the temperature increases the Fermilevel is likely to move closer and closer to E i. So this difference between E f and E v is likely to increase. Basically the assumption that is likely to be violated is the neglect of thermal generation which is the important assumption that we will have to check. (Refer Slide Time: 44:16) Let us do the calculations that 600K. At 600K again neglecting thermal generation and assuming complete impurity ionization you will get p po as same as at 300K and that is 5 into 10 to the power 15 by cm cube. Now, when you want to estimate the n po that is electron concentration you will have to estimate n i at 600K and that is what we do not know. To estimate this we must estimate n i so let us estimate n i at 600K.
18 (Refer Slide Time: 44:48) Here n i at 600K we can estimate in terms of n i at 300K as follows. So n i (600K) by n i (300K) is equal to (600 by 300) power 1.5 exp(minus E g by 2K) into (1 by 600 minus 1 by 300) where we take the 300 out so that 2K(T) corresponding to 300 we know is ev. We can write this part as exp minus E g by 2 into ((300 by 600) minus 1). This is the way you must rewrite the term because now this part can be calculated easily instead of calculating this particular term from Boltzmann constant and the temperature of 300K or simply calculating this term by energy gap and Boltzmann constant and then multiplying by this term, you bring that 300K of room temperature out so that 2KT can be written as Now you simplify this and the result would be 2 into 10 to the power 15 by cm cube. Note that we have substituted this particular term Eg as 1.12eV and when you substitute this as 1.12eV you get 2 into 10 to the power 15 by cm cube. In practice however n i at 600K will be more than this and the actual value will be about 5 into 10 to the power 15 by cm cube if you include the reduction in Eg with temperature so this is a more realistic value. However, we will not use this value but let us continue to use this value where we assume energy gap is 1.12eV. Once you obtain n i now you can estimate n po as 2(10 to the power 15) whole square by 5 into 10 to the power 15 and the result is 8 into 10 to the power 14 by cm cube. Now you see that in this case that the n po is not really very small compared to N a minus N d. In other words, this is definitely more than 1 by 10th of this and thermal generation is not really negligible. In other words we must take into account thermal generation while estimating the majority carrier concentration. In fact as we have said 2 into 10 to the power 15 is an approximate value which neglects the reduction in energy gap at higher temperature. If you take the energy gap reduction in account then n i will be 5 into 10 to the power 15 and then your minority carrier concentration n po will also turn out to be the same as majority carrier concentration therefore it is almost an intrinsic semiconductor.
19 So, in that case how do you take thermal generation into account? Here we write n po is not much less N a minus N d hence thermal generation should be taken into account. (Refer Slide Time: 49:25) So if you want to take that into account then you have to use the quadratic formula that is N a minus N d plus here you will have the n po while calculating p po and that quadratic formula is N a minus N d by 2(1 plus square root of 1 plus 4n i square by (N a minus N d ) whole square. So we have written down this particular relation in a slightly different form earlier. If you substitute the various terms the value will turn out to be 5.7 into 10 to the power 15 by cm cube and then if you calculate n po using this value you will get 7 into 10 to the power 15 by cm cube. So here we have used n i as 2 into 10 to the power 15 by cm cube. This is how one can estimate the carrier concentrations at 600K. As we have said earlier complete impurity ionization is already justified and we need not check Boltzmann approximation because it will be valid. So this is how one can estimate the Fermilevel and the concentration and derive the information that we want about the semiconductor. Now, before we close this topic it is useful to know that all impurities do not behave like boron and phosphorous. Their ionization energies are not so small as 0.045eV. Let us see the different kinds of ionization energies of other impurities in silicon.
20 (Refer Slide Time: 51:22) Here the impurity levels corresponding to different impurities are shown. The impurities shown here are antimony, phosphorous, arsenic, carbon, gold, boron, aluminum and gallium. The positive sign indicates donor impurity or donor level and negative sign is the acceptor level. Further the number here indicates the distance of this particular level from the nearest band edge. So, for example this 0.25 here would mean the distance of this particular carbon level from E c. On the other hand 0.29 here would mean the distance of this particular level associated with gold from E v. Now what you see from this diagram is that some impurities have small ionization energies like antimony, phosphorous, arsenic, boron, aluminum and gallium. So it is donor level close to conduction band edge or acceptor level close to valence band edge. These kinds of impurities can be very useful in changing the carrier concentration because they get ionized very easily and they are used to change the concentration or resistivity of silicon and such impurities are called shallow impurities. On the other hand, you have what are called deep impurities. These are the impurities such as carbon where ionization energy is large. The word deep implies that the impurity is located much inside as compared to the relevant band edge and shallow means it is close to the relevant band edge. So what you see from here is that it is not necessary that donor level should always be close to the conduction band edge. You can have donor level far away from the conduction band edge as it is happening in carbon. And similarly, as it is happening in gold the acceptor impurity is far away from the valence band edge so these are deep impurities. Now what you see further here is that it is not necessary that impurity should give rise to only one level. Here you have carbon which gives rise to two donor levels at two different locations in the energy gap. Finally it is not necessary that an impurity should be only donor type or only acceptor type. Gold introduces both donor level as well as an acceptor level. So impurities which
21 have both types of levels donor and acceptor are called amphoteric impurities. So deep impurities like gold and many others are useful in altering the transient response of the semiconductor and we will see this in our discussion on excess carriers that cannot change the resistivity because their ionization energy is large but they can change the transient response. Now let us quickly summarize the topics we have discussed in these nine lectures on Equilibrium Carrier Concentration. (Refer Slide Time: 55:05) First we covered some basic concepts such as types of semiconductors, then the concept of thermal equilibrium and steady state and the idea of wave particle duality. Then we went on to discuss intrinsic semiconductor wherein we did the bond and band models, generation and recombination phenomena, then the positively charged carrier or the hole concept, what is the effective mass of a carrier, the FermiDirac statistics and Fermilevel.
22 (Refer Slide Time: 55:33) Now this discussion for the intrinsic semiconductor was repeated in a similar manner for extrinsic semiconductors. We discussed the majority and minority carriers, the bond and the band models and the FermiDirac statistics and the Fermilevel. (Refer Slide Time: 55:48) Now it also useful to see some of the properties of semiconductors that we must remember namely the group of the semiconductor, the atomic number, the valence electrons number, the atomic concentration 5 into 10 to the power 22 by cm cube is a very important number, the crystal structure of a semiconductor, the lattice constant and the bond energy.
23 (Refer Slide Time: 56:11) Further the band gap, the electron affinity, the intrinsic concentration at room temperature, effective density of states in conduction valence bands, the dielectric constant and finally the effective masses of electrons and holes under conductivity and density of states situations. (Refer Slide Time: 56:28)
24 (Refer Slide Time: 56:35) Let us also see some constants that we have used and which we must remember. How much is 1 Angstrom in terms of centimeters? How much is a micron in terms of Angstroms? Then what is KT at 300K? How much is 1 electron volt in terms of joules? What is the effective mass of an electron, the permittivity of free space, the velocity of light c the wave length lambda corresponding to 1 electron volt quantum that is 1.24 mm etc. Let us also see the value of the Plank s constant and finally the ionization energy of shallow donors such as phosphorous and boron which are commonly used for doping silicon. The next topic for discussion would be Carrier Transport.
Intrinsic and Extrinsic Semiconductors, FermiDirac Distribution Function, the Fermi level and carrier concentrations
ENEE 33, Spr. 09 Supplement I Intrinsic and Extrinsic Semiconductors, FermiDirac Distribution Function, the Fermi level and carrier concentrations Zeynep Dilli, Oct. 2008, rev. Mar 2009 This is a supplement
More informationDoped Semiconductors. Dr. Katarzyna Skorupska
Doped Semiconductors Dr. Katarzyna Skorupska 1 Doped semiconductors Increasing the conductivity of semiconductors by incorporation of foreign atoms requires increase of the concentration of mobile charge
More informationSemiconductor Physics
10p PhD Course Semiconductor Physics 18 Lectures NovDec 2011 and Jan Feb 2012 Literature Semiconductor Physics K. Seeger The Physics of Semiconductors Grundmann Basic Semiconductors Physics  Hamaguchi
More informationSolidState Physics: The Theory of Semiconductors (Ch. 10.610.8) SteveSekula, 30 March 2010 (created 29 March 2010)
Modern Physics (PHY 3305) Lecture Notes Modern Physics (PHY 3305) Lecture Notes SolidState Physics: The Theory of Semiconductors (Ch. 10.610.8) SteveSekula, 30 March 2010 (created 29 March 2010) Review
More information(Refer Slide Time: 02:55)
MaxwellBoltzmann Distribution vs FermiDirac Distribution Prof. Dr.Prathap Haridoss Department of Metallurgical and Materials Engineering Indian Institute of Technology, Chennai Lecture No. # 20 Hello,
More informationChapter 5. Second Edition ( 2001 McGrawHill) 5.6 Doped GaAs. Solution
Chapter 5 5.6 Doped GaAs Consider the GaAs crystal at 300 K. a. Calculate the intrinsic conductivity and resistivity. Second Edition ( 2001 McGrawHill) b. In a sample containing only 10 15 cm 3 ionized
More informationBasic Electronics Prof. Dr. Chitralekha Mahanta Department of Electronics and Communication Engineering Indian Institute of Technology, Guwahati
Basic Electronics Prof. Dr. Chitralekha Mahanta Department of Electronics and Communication Engineering Indian Institute of Technology, Guwahati Module: 2 Bipolar Junction Transistors Lecture2 Transistor
More informationLecture 2 Semiconductor Physics (I)
Lecture 2 Semiconductor Physics (I) Outline Intrinsic bond model : electrons and holes Generation and recombination Intrinsic semiconductor Doping: Extrinsic semiconductor Charge Neutrality Reading Assignment:
More informationINSTITUTE FOR APPLIED PHYSICS Physical Practice for Learners of Engineering sciences Hamburg University, Jungiusstraße 11
INSTITUTE FOR APPIED PHYSICS Physical Practice for earners of Engineering sciences Hamburg University, Jungiusstraße 11 Hall effect 1 Goal Characteristic data of a test semiconductor (Germanium) should
More informationLecture 8: Extrinsic semiconductors  mobility
Lecture 8: Extrinsic semiconductors  mobility Contents Carrier mobility. Lattice scattering......................... 2.2 Impurity scattering........................ 3.3 Conductivity in extrinsic semiconductors............
More informationThe Physics of Energy sources Renewable sources of energy. Solar Energy
The Physics of Energy sources Renewable sources of energy Solar Energy B. Maffei Bruno.maffei@manchester.ac.uk Renewable sources 1 Solar power! There are basically two ways of using directly the radiative
More information3. Diodes and Diode Circuits. 3. Diodes and Diode Circuits TLT8016 Basic Analog Circuits 2005/2006 1
3. Diodes and Diode Circuits 3. Diodes and Diode Circuits TLT8016 Basic Analog Circuits 2005/2006 1 3.1 Diode Characteristics SmallSignal Diodes Diode: a semiconductor device, which conduct the current
More informationSEMICONDUCTOR I: Doping, semiconductor statistics (REF: Sze, McKelvey, and Kittel)
SEMICONDUCTOR I: Doping, semiconductor statistics (REF: Sze, McKelvey, and Kittel) Introduction Based on known band structures of Si, Ge, and GaAs, we will begin to focus on specific properties of semiconductors,
More informationSample Exercise 12.1 Calculating Packing Efficiency
Sample Exercise 12.1 Calculating Packing Efficiency It is not possible to pack spheres together without leaving some void spaces between the spheres. Packing efficiency is the fraction of space in a crystal
More informationSemiconductors, diodes, transistors
Semiconductors, diodes, transistors (Horst Wahl, QuarkNet presentation, June 2001) Electrical conductivity! Energy bands in solids! Band structure and conductivity Semiconductors! Intrinsic semiconductors!
More informationLecture 2  Semiconductor Physics (I) September 13, 2005
6.012  Microelectronic Devices and Circuits  Fall 2005 Lecture 21 Lecture 2  Semiconductor Physics (I) September 13, 2005 Contents: 1. Silicon bond model: electrons and holes 2. Generation and recombination
More informationCrystalline solids. A solid crystal consists of different atoms arranged in a periodic structure.
Crystalline solids A solid crystal consists of different atoms arranged in a periodic structure. Crystals can be formed via various bonding mechanisms: Ionic bonding Covalent bonding Metallic bonding Van
More informationBasic Quantum Mechanics Prof. Ajoy Ghatak Department of Physics. Indian Institute of Technology, Delhi
Basic Quantum Mechanics Prof. Ajoy Ghatak Department of Physics. Indian Institute of Technology, Delhi Module No. # 02 Simple Solutions of the 1 Dimensional Schrodinger Equation Lecture No. # 7. The Free
More informationCHAPTER 1: Semiconductor Materials & Physics
Chapter 1 1 CHAPTER 1: Semiconductor Materials & Physics In this chapter, the basic properties of semiconductors and microelectronic devices are discussed. 1.1 Semiconductor Materials Solidstate materials
More informationChapter No: 14 Chapter: Semiconductor Electronics: Materials, Devices And Simple Circuits (ONE MARK QUESTIONS)
Chapter No: 14 Chapter: Semiconductor Electronics: Materials, Devices And Simple Circuits (ONE MARK QUESTIONS) 1. What is an electronic device? It is a device in which controlled flow of electrons takes
More informationProbability and Statistics Prof. Dr. Somesh Kumar Department of Mathematics Indian Institute of Technology, Kharagpur
Probability and Statistics Prof. Dr. Somesh Kumar Department of Mathematics Indian Institute of Technology, Kharagpur Module No. #01 Lecture No. #15 Special DistributionsVI Today, I am going to introduce
More informationFYS3410  Vår 2015 (Kondenserte fasers fysikk) http://www.uio.no/studier/emner/matnat/fys/fys3410/v15/index.html
FYS3410  Vår 015 (Kondenserte fasers fysikk) http://www.uio.no/studier/emner/matnat/fys/fys3410/v15/index.html Pensum: Introduction to Solid State Physics by Charles Kittel (Chapters 19 and 17, 18, 0,
More informationLecture  4 Diode Rectifier Circuits
Basic Electronics (Module 1 Semiconductor Diodes) Dr. Chitralekha Mahanta Department of Electronics and Communication Engineering Indian Institute of Technology, Guwahati Lecture  4 Diode Rectifier Circuits
More informationSolid State Detectors = SemiConductor based Detectors
Solid State Detectors = SemiConductor based Detectors Materials and their properties Energy bands and electronic structure Charge transport and conductivity Boundaries: the pn junction Charge collection
More informationDiodes and Transistors
Diodes What do we use diodes for? Diodes and Transistors protect circuits by limiting the voltage (clipping and clamping) turn AC into DC (voltage rectifier) voltage multipliers (e.g. double input voltage)
More informationManagerial Economics Prof. Trupti Mishra S.J.M. School of Management Indian Institute of Technology, Bombay. Lecture  13 Consumer Behaviour (Contd )
(Refer Slide Time: 00:28) Managerial Economics Prof. Trupti Mishra S.J.M. School of Management Indian Institute of Technology, Bombay Lecture  13 Consumer Behaviour (Contd ) We will continue our discussion
More informationElectrical Properties
Electrical Properties Outline of this Topic 1. Basic laws and electrical properties of metals 2. Band theory of solids: metals, semiconductors and insulators 3. Electrical properties of semiconductors
More informationCHAPTER  45 SEMICONDUCTOR AND SEMICONDUCTOR DEVICES
1. f = 101 kg/m, V = 1 m CHAPTER  45 SEMCONDUCTOR AND SEMCONDUCTOR DEVCES m = fv = 101 1 = 101 kg No.of atoms = 101 10 6 10 = 64.6 10 6. a) Total no.of states = N = 64.6 10 6 = 58.5 = 5. 10 8 10 6 b)
More informationENEE 313, Spr 09 Midterm II Solution
ENEE 313, Spr 09 Midterm II Solution PART I DRIFT AND DIFFUSION, 30 pts 1. We have a silicon sample with nonuniform doping. The sample is 200 µm long: In the figure, L = 200 µm= 0.02 cm. At the x = 0
More information5.4 The Quadratic Formula
Section 5.4 The Quadratic Formula 481 5.4 The Quadratic Formula Consider the general quadratic function f(x) = ax + bx + c. In the previous section, we learned that we can find the zeros of this function
More informationSteel Making Prof. Deepak Mazumdar Prof. S. C. Koria Department of Materials Science and Engineering Indian Institute of Technology, Kanpur
Steel Making Prof. Deepak Mazumdar Prof. S. C. Koria Department of Materials Science and Engineering Indian Institute of Technology, Kanpur Module No. # 01 Lecture No. # 10 Modern Steelmaking I, Oxygen
More informationApplied Thermodynamics for Marine Systems Prof. P. K. Das Department of Mechanical Engineering Indian Institute of Technology, Kharagpur
Applied Thermodynamics for Marine Systems Prof. P. K. Das Department of Mechanical Engineering Indian Institute of Technology, Kharagpur Lecture  7 Ideal Gas Laws, Different Processes Let us continue
More informationFigure 1. Diode circuit model
Semiconductor Devices Nonlinear Devices Diodes Introduction. The diode is two terminal non linear device whose IV characteristic besides exhibiting nonlinear behavior is also polarity dependent. The
More informationSoil Dynamics Prof. Deepankar Choudhury Department of Civil Engineering Indian Institute of Technology, Bombay
Soil Dynamics Prof. Deepankar Choudhury Department of Civil Engineering Indian Institute of Technology, Bombay Module  2 Vibration Theory Lecture  8 Forced Vibrations, Dynamic Magnification Factor Let
More informationSemiconductor Detectors Calorimetry and Tracking with High Precision
Semiconductor Detectors Calorimetry and Tracking with High Precision Applications 1. Photon spectroscopy with high energy resolution. Vertex detection with high spatial resolution 3. Energy measurement
More informationRate Equations and Detailed Balance
Rate Equations and Detailed Balance Initial question: Last time we mentioned astrophysical masers. Why can they exist spontaneously? Could there be astrophysical lasers, i.e., ones that emit in the optical?
More informationFieldEffect (FET) transistors
FieldEffect (FET) transistors References: Hayes & Horowitz (pp 142162 and 244266), Rizzoni (chapters 8 & 9) In a fieldeffect transistor (FET), the width of a conducting channel in a semiconductor and,
More informationFall 2004 Ali Shakouri
University of California at Santa Cruz Jack Baskin School of Engineering Electrical Engineering Department EE145L: Properties of Materials Laboratory Lab 5b: Temperature Dependence of Semiconductor Conductivity
More informationLAB IV. SILICON DIODE CHARACTERISTICS
LAB IV. SILICON DIODE CHARACTERISTICS 1. OBJECTIVE In this lab you are to measure IV characteristics of rectifier and Zener diodes in both forward and reversebias mode, as well as learn to recognize
More informationMeasuring Silicon and Germanium Band Gaps using Diode Thermometers
Measuring Silicon and Germanium Band Gaps using Diode Thermometers Haris Amin Department of Physics, Wabash College, Crawfordsville, IN 47933 (Dated: April 11, 2007) This paper reports the band gaps of
More informationThe Electrical Conductivity and Hall Effect of Silicon. Royal Radar Establishment, Malvern, Worcs.
193. The Electrical Conductivity and Hall Effect of Silicon BY E. H. PUTLEY AND W. H. MITCHELL Royal Radar Establishment, Malvern, Worcs. MS. received 27th February 1958, and in final form 18th April 1958
More informationFUNDAMENTAL PROPERTIES OF SOLAR CELLS
FUNDAMENTAL PROPERTIES OF SOLAR CELLS January 31, 2012 The University of Toledo, Department of Physics and Astronomy SSARE, PVIC Principles and Varieties of Solar Energy (PHYS 4400) and Fundamentals of
More informationph. Weak acids. A. Introduction
ph. Weak acids. A. Introduction... 1 B. Weak acids: overview... 1 C. Weak acids: an example; finding K a... 2 D. Given K a, calculate ph... 3 E. A variety of weak acids... 5 F. So where do strong acids
More informationConduction in Semiconductors
Chapter 1 Conduction in Semiconductors 1.1 Introduction All solidstate devices, e.g. diodes and transistors, are fabricated from materials known as semiconductors. In order to understand the operation
More informationObjectives 200 CHAPTER 4 RESISTANCE
Objectives Explain the differences among conductors, insulators, and semiconductors. Define electrical resistance. Solve problems using resistance, voltage, and current. Describe a material that obeys
More informationUnderstanding the pn Junction by Dr. Alistair Sproul Senior Lecturer in Photovoltaics The Key Centre for Photovoltaic Engineering, UNSW
Understanding the pn Junction by Dr. Alistair Sproul Senior Lecturer in Photovoltaics The Key Centre for Photovoltaic Engineering, UNSW The pn junction is the fundamental building block of the electronic
More informationKirchhoff's Rules and Applying Them
[ Assignment View ] [ Eðlisfræði 2, vor 2007 26. DC Circuits Assignment is due at 2:00am on Wednesday, February 21, 2007 Credit for problems submitted late will decrease to 0% after the deadline has passed.
More informationNTC Thermistor theory TABLE OF CONTENTS
NTC Thermistor theory TABLE OF CONTENTS NTC Thermistor Theory................. Chip Configuration............................ Volume Resistivity............................3 Resistance..................................
More informationThe nearlyfree electron model
Handout 3 The nearlyfree electron model 3.1 Introduction Having derived Bloch s theorem we are now at a stage where we can start introducing the concept of bandstructure. When someone refers to the bandstructure
More informationYrd. Doç. Dr. Aytaç Gören
H2  AC to DC Yrd. Doç. Dr. Aytaç Gören ELK 2018  Contents W01 Basic Concepts in Electronics W02 AC to DC Conversion W03 Analysis of DC Circuits W04 Transistors and Applications (HBridge) W05 Op Amps
More informationElectrical Conductivity
Advanced Materials Science  Lab Intermediate Physics University of Ulm Solid State Physics Department Electrical Conductivity Translated by MichaelStefan Rill January 20, 2003 CONTENTS 1 Contents 1 Introduction
More informationChapter 1. Semiconductors
THE ELECTRON IN ELECTRIC FIELDS Semiconductors If we were to take two parallel plates and connect a voltage source across them as shown in Figure 1, an electric field would be set up between the plates.
More informationELECTRICAL CONDUCTION
Chapter 12: Electrical Properties Learning Objectives... How are electrical conductance and resistance characterized? What are the physical phenomena that distinguish conductors, semiconductors, and insulators?
More informationFieldEffect (FET) transistors
FieldEffect (FET) transistors References: Barbow (Chapter 8), Rizzoni (chapters 8 & 9) In a fieldeffect transistor (FET), the width of a conducting channel in a semiconductor and, therefore, its currentcarrying
More informationHIGHER PHYSICS. Electricity. GWC Revised Higher Physics 12/13.
HIGHER PHYSICS Electricity http://blog.enn.com/?p=481 1 GWC Revised Higher Physics 12/13 HIGHER PHYSICS a) MONITORING and MEASURING A.C. Can you talk about: a.c. as a current which changes direction and
More informationForce on Moving Charges in a Magnetic Field
[ Assignment View ] [ Eðlisfræði 2, vor 2007 27. Magnetic Field and Magnetic Forces Assignment is due at 2:00am on Wednesday, February 28, 2007 Credit for problems submitted late will decrease to 0% after
More informationWhy Vedic Mathematics?
Why Vedic Mathematics? Many Indian Secondary School students consider Mathematics a very difficult subject. Some students encounter difficulty with basic arithmetical operations. Some students feel it
More informationOxide. Metal V G. Silicon. Fig.A6.1 MOS capacitor structure
A.6 The MOS capacitor The MOS capacitor consists of a metaloxidesemiconductor layer structure which forms a voltage dependent capacitor. This particular structure has been studied extensively because
More informationNORGES TEKNISK NATURVITENSKAPELIGE UNIVERSITET INSTITUTT FOR FYSIKK. Eksamen i Emne TFY4220 Faste Stoffers Fysikk
Page of 5 NORGES TEKNISK NATURVITENSKAPELIGE UNIVERSITET INSTITUTT FOR FYSIKK Fagleg kontakt under eksamen: Institutt for fysikk, Gløshaugen Professor Steinar Raaen, 4896758 Eksamen i Emne TFY40 Faste
More informationSemiconductor doping. Si solar Cell
Semiconductor doping Si solar Cell Two Levels of Masks  photoresist, alignment Etch and oxidation to isolate thermal oxide, deposited oxide, wet etching, dry etching, isolation schemes Doping  diffusion/ion
More information2. THE xy PLANE 7 C7
2. THE xy PLANE 2.1. The Real Line When we plot quantities on a graph we can plot not only integer values like 1, 2 and 3 but also fractions, like 3½ or 4¾. In fact we can, in principle, plot any real
More informationFluid Mechanics Prof. T. I. Eldho Department of Civil Engineering Indian Institute of Technology, Bombay. Lecture No. # 36 Pipe Flow Systems
Fluid Mechanics Prof. T. I. Eldho Department of Civil Engineering Indian Institute of Technology, Bombay Lecture No. # 36 Pipe Flow Systems Welcome back to the video course on Fluid Mechanics. In today
More informationHigh Open Circuit Voltage of MQW Amorphous Silicon Photovoltaic Structures
High Open Circuit Voltage of MQW Amorphous Silicon Photovoltaic Structures ARGYRIOS C. VARONIDES Physics and EE Department University of Scranton 800 Linden Street, Scranton PA, 18510 United States Abstract:
More informationUnit 12 Practice Test
Name: Class: Date: ID: A Unit 12 Practice Test Multiple Choice Identify the choice that best completes the statement or answers the question. 1) A solid has a very high melting point, great hardness, and
More informationCharacteristic curves of a solar cell
Related Topics Semiconductor, pn junction, energyband diagram, Fermi characteristic energy level, diffusion potential, internal resistance, efficiency, photoconductive effect, acceptors, donors, valence
More informationUntitled Document. 1. Which of the following best describes an atom? 4. Which statement best describes the density of an atom s nucleus?
Name: Date: 1. Which of the following best describes an atom? A. protons and electrons grouped together in a random pattern B. protons and electrons grouped together in an alternating pattern C. a core
More informationSession 7 Bivariate Data and Analysis
Session 7 Bivariate Data and Analysis Key Terms for This Session Previously Introduced mean standard deviation New in This Session association bivariate analysis contingency table covariation least squares
More informationExponents and Radicals
Exponents and Radicals (a + b) 10 Exponents are a very important part of algebra. An exponent is just a convenient way of writing repeated multiplications of the same number. Radicals involve the use of
More informationLow Power VLSI Circuits and Systems Prof. Pro. Ajit Pal Department of Computer Science and Engineering Indian Institute of Technology, Kharagpur
Low Power VLSI Circuits and Systems Prof. Pro. Ajit Pal Department of Computer Science and Engineering Indian Institute of Technology, Kharagpur Lecture No. # 14 Pass Transistor Logic Circuits  I Hello
More informationPartial Fractions. Combining fractions over a common denominator is a familiar operation from algebra:
Partial Fractions Combining fractions over a common denominator is a familiar operation from algebra: From the standpoint of integration, the left side of Equation 1 would be much easier to work with than
More informationGuide to SRW Section 1.7: Solving inequalities
Guide to SRW Section 1.7: Solving inequalities When you solve the equation x 2 = 9, the answer is written as two very simple equations: x = 3 (or) x = 3 The diagram of the solution is 65 43 21 0
More informationLecture 2: Semiconductors: Introduction
Lecture 2: Semiconductors: Introduction Contents 1 Introduction 1 2 Band formation in semiconductors 2 3 Classification of semiconductors 5 4 Electron effective mass 10 1 Introduction Metals have electrical
More informationThe MaxwellBoltzmann Distribution
The MaxwellBoltzmann Distribution Gases are composed of atoms or molecules. These atoms or molecules do not really interact with each other except through collisions. In many cases, we may think of a
More informationphys4.17 Page 1  under normal conditions (pressure, temperature) graphite is the stable phase of crystalline carbon
Covalent Crystals  covalent bonding by shared electrons in common orbitals (as in molecules)  covalent bonds lead to the strongest bound crystals, e.g. diamond in the tetrahedral structure determined
More informationPSS 17.1: The Bermuda Triangle
Assignment 6 Consider 6.0 g of helium at 40_C in the form of a cube 40 cm. on each side. Suppose 2000 J of energy are transferred to this gas. (i) Determine the final pressure if the process is at constant
More informationc 2008 Je rey A. Miron We have described the constraints that a consumer faces, i.e., discussed the budget constraint.
Lecture 2b: Utility c 2008 Je rey A. Miron Outline: 1. Introduction 2. Utility: A De nition 3. Monotonic Transformations 4. Cardinal Utility 5. Constructing a Utility Function 6. Examples of Utility Functions
More information(Refer Slide Time: 2:03)
Control Engineering Prof. Madan Gopal Department of Electrical Engineering Indian Institute of Technology, Delhi Lecture  11 Models of Industrial Control Devices and Systems (Contd.) Last time we were
More informationName Partners Date. Energy Diagrams I
Name Partners Date Visual Quantum Mechanics The Next Generation Energy Diagrams I Goal Changes in energy are a good way to describe an object s motion. Here you will construct energy diagrams for a toy
More informationHeat Transfer Prof. Dr. Aloke Kumar Ghosal Department of Chemical Engineering Indian Institute of Technology, Guwahati
Heat Transfer Prof. Dr. Aloke Kumar Ghosal Department of Chemical Engineering Indian Institute of Technology, Guwahati Module No. # 02 One Dimensional Steady State Heat Transfer Lecture No. # 05 Extended
More informationBASIC ELECTRONICS TRANSISTOR THEORY. December 2011
AM 5204 BASIC ELECTRONICS TRANSISTOR THEORY December 2011 DISTRIBUTION RESTRICTION: Approved for Public Release. Distribution is unlimited. DEPARTMENT OF THE ARMY MILITARY AUXILIARY RADIO SYSTEM FORT
More informationDiode Characteristics
by Kenneth A. Kuhn Oct. 3, 2007, rev. Sept. 3, 2009, draft more to come Introduction This paper examines various electrical characteristics of a typical silicon junction diode. Useful mathematical relations
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationData Communications Prof. Ajit Pal Department of Computer Science & Engineering Indian Institute of Technology, Kharagpur Lecture # 03 Data and Signal
(Refer Slide Time: 00:01:23) Data Communications Prof. Ajit Pal Department of Computer Science & Engineering Indian Institute of Technology, Kharagpur Lecture # 03 Data and Signal Hello viewers welcome
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationSolving Quadratic Equations
9.3 Solving Quadratic Equations by Using the Quadratic Formula 9.3 OBJECTIVES 1. Solve a quadratic equation by using the quadratic formula 2. Determine the nature of the solutions of a quadratic equation
More information1.6 The Order of Operations
1.6 The Order of Operations Contents: Operations Grouping Symbols The Order of Operations Exponents and Negative Numbers Negative Square Roots Square Root of a Negative Number Order of Operations and Negative
More information5.1 Radical Notation and Rational Exponents
Section 5.1 Radical Notation and Rational Exponents 1 5.1 Radical Notation and Rational Exponents We now review how exponents can be used to describe not only powers (such as 5 2 and 2 3 ), but also roots
More informationSemiconductor pn junction diodes
Semiconductor pn junction diodes p n pn junction formation ptype material Semiconductor material doped with acceptors. Material has high hole concentration Concentration of free electrons in ptype
More informationCh. 14 The Periodic Table p. 390406
Name Period PREAP 141 Development of the Periodic Table Ch. 14 The Periodic Table p. 390406 Dmitri Mendeleev published the first periodic table in 1869. He organized the elements by atomic mass. He
More informationRefrigeration and Air Conditioning Prof. M. Ramgopal Department of Mechanical Engineering Indian Institute of Technology, Kharagpur
Refrigeration and Air Conditioning Prof. M. Ramgopal Department of Mechanical Engineering Indian Institute of Technology, Kharagpur Lecture No. # 18 Worked Out Examples  I Welcome back in this lecture.
More informationChapter 2 Formulas and Decimals
Chapter Formulas and Decimals Section A Rounding, Comparing, Adding and Subtracting Decimals Look at the following formulas. The first formula (P = A + B + C) is one we use to calculate perimeter of a
More information7.6 Approximation Errors and Simpson's Rule
WileyPLUS: Home Help Contact us Logout HughesHallett, Calculus: Single and Multivariable, 4/e Calculus I, II, and Vector Calculus Reading content Integration 7.1. Integration by Substitution 7.2. Integration
More informationUnits and Dimensions in Physical Chemistry
Units and Dimensions in Physical Chemistry Units and dimensions tend to cause untold amounts of grief to many chemists throughout the course of their degree. My hope is that by having a dedicated tutorial
More informationFree Electron Fermi Gas (Kittel Ch. 6)
Free Electron Fermi Gas (Kittel Ch. 6) Role of Electrons in Solids Electrons are responsible for binding of crystals  they are the glue that hold the nuclei together Types of binding (see next slide)
More informationPhysics Lab Report Guidelines
Physics Lab Report Guidelines Summary The following is an outline of the requirements for a physics lab report. A. Experimental Description 1. Provide a statement of the physical theory or principle observed
More informationAppendix A: Science Practices for AP Physics 1 and 2
Appendix A: Science Practices for AP Physics 1 and 2 Science Practice 1: The student can use representations and models to communicate scientific phenomena and solve scientific problems. The real world
More informationWEAK ACIDS AND BASES
WEAK ACIDS AND BASES [MH5; Chapter 13] Recall that a strong acid or base is one which completely ionizes in water... In contrast a weak acid or base is only partially ionized in aqueous solution... The
More informationCALCULATIONS & STATISTICS
CALCULATIONS & STATISTICS CALCULATION OF SCORES Conversion of 15 scale to 0100 scores When you look at your report, you will notice that the scores are reported on a 0100 scale, even though respondents
More informationLecture 3: Optical Properties of Bulk and Nano. 5 nm
Lecture 3: Optical Properties of Bulk and Nano 5 nm First H/W#1 is due Sept. 10 Course Info The Previous Lecture Origin frequency dependence of χ in real materials Lorentz model (harmonic oscillator model)
More informationCopyright Page 1
1 Introduction to Bonding: TwoDimensional Lewis tructures Key Terms: abbreviated electron configuration combines the inert, noble core electrons (abbreviated via a noble element) with the outermost or
More information